N ANOSTRUCTURES FOR T HERAPY AND
R OSARIA A RUTA
In partial Fulfillment of the Requirements for the Degree of Doctor of Philosophy in Engineering Materials and Structures at the Federico II
University for Naples
Prof. Paolo Antonio Netti
Dr. Ing. Enza Torino
Prof. Giuseppe Mensitieri
3 EXTENDED ABSTRACT
The preparation of Nanostructures of desired shape, composition and with tailored properties is of wide scientific and technological interest. Indeed, a variety of nanoparticle architectures have been proposed as nanocarriers, these include liposomes, quantum dots (QD), gold-nanoshells, mesoporous materials, micelles, magnetic nanoparticles, dendrimers, and Carbon Nanotubes (CNTs) as so as several materials have been studied for use in active agents targeting. Among them, as asserted by different authors, hollow biopolymeric nanocapsules or (nanoencapsulated systems) as active substance carriers, compared to other particulated systems, show higher drug encapsulation efficiency due to optimized drug solubility in the core, low polymeric content compared such as to nanospheres, drug polymeric shell protection against degradation factor like pH and light and the reduction of tissue irritation due to the polymeric shell.
Several research teams have extensively studied the nanoparticles formation mechanism, and generally there are several classical methods for the preparation of nanocapsular systems:
nanoprecipitation, emulsion diffusion, emulsion evaporation, double emulsification, emulsion coacervation, polymer coating and layer by layer.
4 Despite the fact the research proposed on these methods has shown important strategies, all these methods present critical challenges with a view of the industrial development. Indeed, it is important to take into account that the method chosen should also considerer other aspects such as active substance stability under operational conditions, particularly stirring, encapsulation efficiency, method feasibility, the generation of contaminants and the need for subsequent purification steps, solvent nature, the water volume required and time consumption. Likewise, the feasibility of scaling-up and cost should be considered.
In these perspectives, to overcome some limitations of traditional processes in nanocapsular structure productions, such as sufficient scale-up to produce the cost reduction required to target volume markets and more complicated procedure not suitable to be industrialized, we focused our attention on the three main approaches:
- the first one based on the Thermally Induced Phase Separation (TIPS) to produce nanocapsules for therapy
- the second one related to the study of the micellization of block- copolymer to apply in the field of enhanced MRI
- the last is the combining of the previous approaches by providing the deposition of the block-copolymer on the surface of the obtained nanocapsules.
5 In the first part of the thesis, we developed a novel approach based on the thermodynamics of Thermally Induced Phase Separation (TIPS) to produce semicrystalline nanocapsules.
Thermally Induced Phase Separation has extensively been used to fabricate various porous biodegradable scaffolds suitable for tissue engineering and drug delivery, even though it has never been studied neither to produce nanocapsules nor to produce semicrystalline nanocapsules. Because of the variety of parameters involved in TIPS process, such as types of polymers, polymer concentration, solvent/nonsolvent ratio, and quenching temperature, we individuate in this approach the possibility to create a value added process enables to overcome the issues related to the production of the nanocapsular systems even by preserving fundamental architectural properties.
In this process, we started by a Poly-L-Lactic Acid (PLLA), a biopolymer largely studied by TIPS. PLLA is a Food&Drug Administration Approved polymer and it is biocompatible and biodegradable material which undergoes scission in the body to monomeric units of lactic acid as a natural intermediate in carbohydrate metabolism. The work also investigates thermodynamic parameters involved in the process able to induce for the first time simultaneously bending and crystallization of polymeric chain to form a nanocapsule. An explanation of this unusual crystallization phenomenon will be described in term of
6 nanoscopic confinement of long flexible chain. Knowledge of the phase behavior of confined long flexible chain is a prerequisite to support the current interest in the construction of nanoscopic devices as so in conﬁnement altering the statistical mechanical properties of DNA.
In the second part of the thesis a Block copolymers of poly lactic acid (PLA) and polyethylene glycol (PEG) has been studied.
Block copolymer are few of the commonly used polymers with hydrophilic and hydrophobic blocks which allows the formation of a stable nano-particulate suspension in an aqueous solvent, where PLA chains predominantly form the core and PEG chains are located outside. A systematic variation in their chemical structure, composition, size, and architecture; block copolymers offer advantages in tuning their shape and functionality in comparison to conventional amphiphiles such as low molecular weight surfactants and lipids. In particular, Diblock PLA-PEG copolymers and triblock PLA-PEG-PLA copolymers allow modulation of the biodegradation rate, the hydrophilicity, and the mechanical properties of the copolymers. Herein we present temperature/time-reliant self- assembly driven simple approach for the development of biocompatible nanostructures for MRI. Endeavor of the present research was to develop Gd loaded PLA-PEG-PLA NPs as the molecular MRI contrast agents to efficiently target tumor. A low molecular PLA-PEG-PLA have been designated to prepare well-
7 demarcated NPs through optimization of kinetics of the self- assembly viz a viz temperature/time/concentration. The hydrophobic/hydrophilic moieties of block copolymer nanoparticles (BCN) were employed to adsorb GD+3 at the surface of BCNs to achieve multifunctional biodegradable NPs for MRI. The paramagnetic properties of the BCNs designed here compare sympathetically with Gd-based agents that have previously been reported. For example, while relaxivity of the commercial products, such Magnevist is of 4 mM-1 sec-1, our micelles can reach relaxivitry of around 30 mM-1 sec-1 , indicating a relaxivity significantly higher than the common paramagnetic contrast agents.
Last part of the thesis has been devoted to the combination of the previous obtained structures in order to apply these new nanostructures in the theranostic field. For this reason only some Caolrimetric studies were performed. Nano-Isothermal Calorimetry (NanoITC) was used to evaluate the deposition of the block on the surface of the nanoparticles while Differential Scanning Calorimetry was used to show the melting properties of the combined system.
Peer Reviewed Paper
Nanocapsules production by Thermally Induced Phase Separation in a nanoconfinement – Rosaria Aruta, Enza Torino, Paolo Antonio Netti
Submitted to Biomaterials
Aqueous Channel Manifestation amongst Biodegradable nanomaterials for favorable Gadolinium entrapping – Rosaria Aruta, Pankaj Thakur, Enza Torino, Paolo Antonio Netti
Submitted to International Journal of Nanomedicine
Nanocapsules decoration by tri-block copolymer and study of their behavior in the theranostic field
Paper in preparation
TABLES OF CONTENTS
EXTENDED ABSTRACT ...3
Peer Reviewed Paper ... 8
CHAPTER I: INTRODUCTION ... 11
NANOPARTICLE FOR THERAPY AND DIAGNOSTIC: ARCHITECTURE AND FEATURES 11 PRODUCTION OF NANOCAPSULES: METHODS, ADVANTAGES AND DRAWBACKS .. 21
AIM OF THE WORK ... 37
REFERENCES ... 38
CHAPTER II: NANOCAPSULES PRODUCTION BY THERMALLY INDUCED PHASE SEPRATION IN A NANOCONFINEMENT... 41
INTRODUCTION ... 41
MATERIALS ... 42
METHODS ... 43
MORPHOLOGICAL AND STRUCTURAL CHARACTERIZATION ... 50
RESULTS ... 56
OPTIMIZATION OF ULTRASONICATION PARAMETERS ... 56
EFFECT OF HIGH PRESSURE HOMOGENIZATION ... 58
EFFECT OF COOLING RATE ON THE FINAL MORPHLOGY ... 61
PURIFICATION AND RECOVERY ... 69
MORPHOLOGICAL CHARACTERIZATION OF NANOCAPSULES ... 73
CRYSTALLINITY BEHAVIOR OF THE PRODUCED NANOCAPSULES... 77
LOADING CAPABILITY AND RELEASE MECHANISM ... 85
THERMODYNAMIC INTERPRETATION OF THE PROCESS ... 88
REFERENCES ... 94
10 CHAPTER III: AQUEOUS CHANNEL MANIFESTATION AMONGST BIODEGRADABLE NANOMATERIALS FOR FAVORABLE
GADOLINIUM ENTRAPPING ... 99
INTRODUCTION ... 99
MATERIALS AND METHOD ... 103
Results and Discussion ... 107
CHAPTER IV: PRELIMINARY DATA ON DEPOSITION OF BLOCK COPOLYMER ON NANOCAPSULAR STRUCTURES TO BE APPLIED IN THE THERANOSTIC FIELD ... 131
INTRODUCTION ... 131
MATERIALS AND METHOD... 131
Materials ... 131
Methods ... 132
RESULTS ... 135
CONCLUSIONS AND PERSPECTIVES ... 138
11 CHAPTER I: INTRODUCTION
NANOPARTICLE FOR THERAPY AND DIAGNOSTIC:
ARCHITECTURE AND FEATURES
Theranostic is an emerging and promising field of the nanomedicine that has captured the interest of researchers because its purpose is to diagnose and treat the diseases at their earliest stage, when the diseases are most likely curable or at least treatable1. To achieve this, it takes advantage of the high capacity of nanoparticles, submicron sized colloidal particles with sizes ranging from 10-1000 nm in diameter, to ferry cargo and loads onto them both imaging and therapeutic functions. Thus, nanoparticle technologies are significantly impacting on the development of both therapeutic and diagnostic agents for simultaneous drug delivery and molecular imaging.
From the point of view of Drug delivery, nanoparticle objective is the delivery of a medicine to its site of therapeutic action because this is one of the main limitations of pharmaceutical and biotechnology industries2. Indeed, most of the drugs are limited by their poor solubility, high toxicity and dosage, aggregation due to poor solubility, nonspecific delivery, in vivo degradation and short circulating half-lives. Thus, nanoparticles have the potential to overcome this limitations and could improve the process of releasing of a bioactive agent at a specific rate and at a specific site, allowing to
12 exploit thousands of new therapeutics that are limited by a safe and effective drug-delivery system.
Although nanoparticles have been developed for a myriad of important diseases, the thrust of research has been focused on solid tumors, cardiovascular diseases, and immunological diseases. In particular, as drug carriers for chemotherapeutics, nanoparticles can be used to deliver medication directly to the tumor while sparing healthy tissue, by bringing several advantages over conventional chemotherapy3, because they can:
• Protect drugs from being degraded in the body before they reach their target;
• Enhance drug absorption into tumors and the cancerous cells themselves;
• Allow for better control over the timing and distribution of drugs to the tissue, making it easier for oncologists to assess how well they work;
• Prevent drugs from interacting with normal cells, thus avoiding side effects.
Along with drug delivery researches other studies have been done for diagnostic applications. In particular, for molecular imaging, that allows the characterization of biological processes at the cellular and subcellular levels in intact organism by exploiting specific molecular probes or contrast agents, most of the contrast agents currently in use consist of low molecular weight compounds that are non-specific, thus making the quantification of disease at early stage difficult4. So,
13 the development of nanoparticulate-based contrast agents could offers a platform to enhance tissue specificity and sensitivity required for in vivo molecular imaging with a minimal administration of the contrast agent.
One significant challenge for the successful development of therapeutic nanoparticles is rapid clearance during systemic delivery5. When nanoparticles enter the bloodstream, the particle surface may experience nonspecific protein adsorption (opsonization), thereby making them more visible to phagocytic cells.
After opsonization, nanoparticles could be rapidly cleared from the bloodstream through phagocytosis by the reticuloendothelial system (RES) in the liver and by spleen filtration. Therefore, the factors that could affect the clearance and biodistribution of nanoparticles, such as particle physicochemical properties and targeting ligand functionalization, should be carefully considered for the optimal design of therapeutic nanoparticles. On the basis of physiological parameters such as hepatic filtration, tissue extravasation/diffusion, and kidney excretion, it is clear that particle size plays a key factor in the long circulation and biodistribution of nanoparticles. Indeed, nanoparticles smaller than 10 nm can be rapidly cleared by the kidneys or through extravasation, while larger nanoparticles may have higher tendency to be cleared by cells of reticuloendothelial system (RES). Moreover, It was observed that nanoparticles <100 nm have a higher potential to circulate in the blood for long periods of time and experience reduced hepatic filtration. Nanoparticle size also
14 plays a key role in tumor accumulation through the EPR effect (Enhanced Permeability and Retention effect)6. This is a phenomenon due to the unique anatomical and pathophysiological characteristics of solid tumor. Namely, in contrast to normal tissues and organs, most solid tumors show a higher vascular density, and tumors blood vessels present defective architecture, such as large gap between endothelial cells (e.g., ~ 1μm), lack of smooth muscle layers, so that macromolecules will have the opportunity to escape from tumor blood vessels and accumulate selectively in tumor tissues, whereas they could not cross normal blood vessels which will result in less side effects. In addition, defected lymphatic function that is important for the recovery of macromolecules in tissues is always found in tumor tissues. Consequently, once macromolecules accumulate in tumor tissues, they will not be cleared from tumor tissues but retain there for long time. Several studies have tried to determine the gap size in the leaky vasculature that depends on the kind of tumor considered. Therefore, to capitalize on the EPR effect and to efficiently escape from the physiological barriers, many studies advocate the optimal nanoparticle size range of approximately 10–250 nm.
It has been established that the surface charge of nanoparticles is another important property because it could affect their uptake by the RES cells7. Neutrally charged particles have demonstrated much lower opsonization rates than charged particles. It was found that positively charged nanoparticles generate a higher immune response
15 compared to neutral or negatively charged nanoparticle formulations. For example, nanoparticles with a primary amine at the surface promote higher rates of phagocytic uptake when compared to those having sulfate, hydroxyl, or carboxyl groups at the surface.
Many studies suggest that the optimal range of nanoparticle surface charge should be between −10 and +10 mV for reduced phagocytosis and minimized nonspecific interactions of nanoparticles. Surface modification of nanoparticles with PEG, which has favorable intrinsic physicochemical properties (e.g., high flexibility and hydrophilicity, low toxicity and immunogenicity), was found to reduce nanoparticle accumulation in off-target organs such as liver and spleen8. A PEG decoration on the nanoparticle’s surface shields hydrophobic or charged particles from being attacked by blood proteins, leading to prolonged circulation half-life compared to non-PEGylated nanoparticles. The length, shape, and density of PEG chains on the nanoparticle surface largely affect its surface hydrophilicity and phagocytosis.
Until now, different architectures of nanoparticles have been developed using a variety of materials including lipids (liposomes), organometallic compound (nanotubes) and polymers (micelles, dendrimers and polymeric nanoparticles)9.
Figure 1. Different architectures applied in the nanomedicine field
Liposomes are artificial, single, or multilaminar vesicles made with bilayered membrane structures with inner aqueous phases, composed of natural or synthetic amphiphilic lipid molecules. They are versatile and tunable vehicles for drug delivery and imaging.
Liposomes exhibit several unique properties including favorable safety profiles, long systemic circulation half-life, and ease of surface modifications. Among the clinically validated nanotechnology products, liposomal drugs were the first nanotherapeutics to get FDA approval for clinical use. Upon intravenous injection, these nanoparticles are rapidly cleared from the bloodstream by the reticuloendothelial defence mechanism, regardless of particle composition. Moreover, instability of the carrier and burst drug release, as well as non-specific uptake by the mononuclear
17 phagocytic system (MPS), provides additional challenges for translating these carriers to the clinic. Other challenges facing the use of liposomes in the clinic include the high production cost, fast oxidation of some phospholipids, and lack of controlled-release properties of encapsulated drugs.
Micellar nanoparticles are attractive structures for carriers of drug and contrast agents because they can form relatively uniform size structures. They can be prepared by self-assembly of a variety of amphiphilic materials that, in aqueous environments, under certain concentrations and temperature, spontaneously self-assemble into core-shell nanostructure, with a hydrophobic core and a hydrophilic shell. This architecture increases the solubility of hydrophobic molecules, and allows incorporating multiple functionalities into a single structure. Polymeric micelles represent a class of micelles that are formed of block copolymers consisting of a hydrophobic block that forms the micellar core, and a hydrophilic portion that forms the corona. This corona (commonly consisting of PEG or equivalent hydrophilic polymer) confers these micelles with biocompatibility, stealth-like properties, and a platform for functionalization.
Dendrimers are polymeric molecules composed of multiple perfectly branched monomers that emanate radially from the central core,
18 thus forming a tree-like structure. They consist of three critical architectural domains: (i) the multivalent surface, containing a larger number of potentially reactive sites, (ii) the interior shells (i.e., branch cell layers defined by dendrons) surrounding the core, and (iii) the core to which the dendrons are attached. These three domains can be tailored to serve various purposes, such as dendritic sensors, drug, contrast agent and gene carriers, or themselves as drugs. They have shown promise for biomedical applications because they (1) can be easily conjugated with targeting molecules, imaging agents, and drugs, (2) have high water solubility and well-defined chemical structures, (3) are biocompatible, and (4) are rapidly cleared from the blood through the kidneys, made possible by their small size (<5 nm), which eliminates the need for biodegradability. Furthermore the end groups of dendrimers can also be modulated to alter dendrimers’
solubility; for instance, the hydrophilic end groups can make a dendrimer with a hydrophobic core water soluble, whereas hydrophobic peripheral moieties can make a dendrimer with a hydrophilic interior soluble in oil. Although promising, dendrimers are more expensive than other nanoparticles and require many repetitive steps for synthesis, posing a challenge for large-scale production.
Carbon nanotubes (CNTs) consist exclusively of carbon atoms arranged in tubular structure. This novel artificial nanomaterial belongs to the family of fullerenes, the third allotropic form of
19 carbon . Based on the number of layers, structures of CNTs are classified into two types: single-walled carbon nanotubes (SWCNTs) and multiwalled carbon nanotubes (MWCNTs). SWCNTs consist of a single graphene cylinder with diameter varying between 0.4 and 2 nm, and usually occur as hexagonal close-packed bundles. MWCNTs consist of two to several coaxial cylinders, each made of a single graphene sheet surrounding a hollow core. CNTs are not soluble in aqueous solutions because they have highly hydrophobic surfaces.
Surface functionalization is required to solubilize CNTs, and to make them biocompatible and low toxic for their medical applications.
They are being investigated as theranostic nanoparticles because of their tunable properties and ability to incorporate multiple functionalities. Many studies have confirmed CNTs to be effective carriers of therapeutics and imaging agent in vitro, however, in vivo studies have led to concerns regarding the associated toxicities. So, the primary barriers that must be overcome include route of biodegradation and reduction of off-target toxicity.
Polymers are the most commonly explored materials for constructing nanoparticles-based drug carriers. Most polymeric nanoparticles are biodegradable and biocompatible, moreover, they exhibit a good potential for surface modification and functionalization with different ligands, provide excellent pharmacokinetic control and are suitable to encapsulate and deliver a plethora of therapeutic agents. The main
20 advantage of using polymeric nanoparticles for drug-delivery applications is their small size when taken up by cells, which could allow efficient drug accumulation at the target sites. Biodegradable materials used for their formulation allow sustained drug release within the target site over a period of days or even weeks.
For preparation of nanoparticles is possible to use both natural hydrophilic polymer and synthetic hydrophobic polymer. Natural hydrophilic polymers such as proteins (gelatine, albumin, lecithin) and polysaccharides (alginate, dextran, chitosan) are widely used. But these polymers have certain disadvantages such as poor batch‑to‑
batch reproductivity, poor mechanical properties, limited residence time (fast degradation and absorption), and potential antigenicity.
Synthetic hydrophobic polymers are characterized by low production costs, and it is possible to design them to obtain the desired chemical-physical properties. They are divided into two groups: The first group includes polyesters (poly (€‑caprolactone), poly(lactic acid), poly (lactide‑co‑glycolide), polystyrene) and the second group includes poly (alkyl cyanoacrylates) (poly (isobutyl cyanoacrylates), poly (butylcyanoacrylates), poly methyl (methcyanoacrylates)).
Nanoparticles can be produced in two different approaches, by polymerization of the monomer or by the preformed polymer. The second case is preferable because the chemical/physical properties of the polymer are already well defined. Depending on the process
21 used for nanoparticles preparation, we can obtain nanospheres or nanocapsules.
Figure 2: In this image the difference between nanoparticles and nanospheres as so between drug encapsulation and absorption is showed.
Nanospheres are matrix particles, i.e., particles whose entire mass is solid and molecules may be adsorbed at the sphere surface or entrapped within the particle matrix. In general, they are spherical, but “nanospheres” with a nonspherical shape are also described in the literature. Nanocapsules are vesicular systems, acting as a kind of reservoir, in which the encapsulated substances are confined to a cavity consisting of a liquid core (either oil or water) surrounded by a solid material shell.
PRODUCTION OF NANOCAPSULES: METHODS, ADVANTAGES AND DRAWBACKS
Nanocapsules can be defined as nano-vesicular systems that exhibit a typical core-shell structure in which the drug is confined to a
22 reservoir or within a cavity surrounded by a polymer membrane or coating10. The cavity can contain the active substance in liquid or solid form or as a molecular dispersion. Likewise, this reservoir can be lipophilic or hydrophobic according to the preparation method and raw materials used. Also, taking into account the operative limitations of preparation methods, nanocapsules can also carry the active substance on their surfaces or imbibed in the polymeric membrane.
Generally, there are six classical methods for the preparation of nanocapsules: nanoprecipitation, emulsion–diffusion, double emulsification, emulsion-coacervation, polymer-coating and layer-by- layer.
Nanoprecipitation (Solvent displacement) method
The nanoprecipitation method is also called solvent displacement11. In this method, the nanocapsule synthesis needs both solvent and non-solvent phases. The solvent phase consists of a solution in a solvent or in a mixture of solvents (i.e. ethanol, acetone, hexane, methylene chloride or dioxane) of a film-forming substance such as a polymer (synthetic, semi-synthetic or naturally occurring polymer), the drug, oil and lipophilic surfactants. On the other hand, the non- solvent phase consisting of a non-solvent or a mixture of non- solvents for the film-forming substance, supplemented with one or more naturally occurring or synthetic surfactants. In most cases, the solvent and non-solvent phases are called organic and aqueous phases, respectively. As a general tendency, the solvent is an organic
23 medium, while the non-solvent is mainly water. However, it is possible to use either two organic phases or two aqueous phases as long as solubility, insolubility and miscibility conditions are satisfied.
In the nanoprecipitation method, the nanocapsules are obtained as a colloidal suspension formed when the organic phase is added slowly and with moderate stirring to the aqueous phase.
The key variables of the procedure are those associated with the conditions of adding the organic phase to the aqueous phase, such as organic phase injection rate, aqueous phase agitation rate, the method of organic phase addition and the organic phase/aqueous phase ratio. Likewise, nanocapsule characteristics are influenced by the nature and concentration of their components. Different theories have been developed to explain the mechanism of nanocapsules formation using this technique. The first is based on Sugimoto’s theory on polymer precipitation that indicated three stages for the process of particle formation in the nanoprecipitation: nucleation, growth and aggregation. The rate of each step determines the particle size and the driving force of these phenomena is supersaturation, which is defined as the ratio of polymer concentration over the solubility of the polymer in the solvent mixture. The separation between the nucleation and the growth stages is the key factor for uniform particle formation. Ideally, operating conditions should allow a high nucleation rate strongly dependent on supersaturation and low growth rate. The second theory is based on Gibbs–Marangoni effect, that explained rapid
24 nanoparticle formation as a process due to differences in surface tension, since a liquid with a high surface tension (aqueous phase) pulls more strongly on the surrounding liquid than one with a low surface tension (organic phase solvent). These differences between surface tensions cause interfacial turbulence and thermal inequalities in the system, leading to the continuous formation of eddies of solvent at the interface of both liquids. Consequently, violent spreading is observed due to mutual miscibility between the solvents, the solvent flows away from regions of low surface tension and the polymer tends to aggregate on the oil surface and forms nanocapsules. According to this explanation, nanocapsule formation is due to polymer aggregation in stabilized emulsion droplets, while apparently the nucleation and growth steps are not involved.
In emulsion-diffusion method12 the experimental procedure performed to achieve this requires three phases: organic, aqueous and dilution. In particular, the encapsulating polymer is dissolved in the organic phase that contain a partially water soluble solvent, saturated with water to ensure the initial thermodynamic equilibrium of both liquids, the active substance and oil. The aqueous phase is an aqueous dispersion of a stabilizing agent, prepared using water saturated with solvent, while the dilution phase is usually water.
For preparation of nanocapsules using the emulsion–diffusion method, the organic phase is emulsified under vigorous agitation in the aqueous phase.
25 The subsequent addition of water to the system causes the diffusion of the solvent into the external phase, resulting in nanocapsule formation. This can be eliminated by distillation or cross-flow filtration depending on the boiling point of the solvent. It has been shown that nanocapsule size is related to the shear rate used in the emulsification process, the chemical composition of the organic phase, the polymer concentration, the oil-to-polymer ratio and the drop size of the primary emulsion. The nanocapsule formation mechanism is based on the theory that each emulsion droplet produces several nanocapsules and that these are formed by the combination of polymer precipitation and interfacial phenomena during solvent diffusion. It is important to note that the interface between organic and aqueous phases was subjected to shear force during the emulsification step. Thus, for the emulsification–diffusion method it might be expected that surface tension gradients can be due to the thermal effects associated with heat transport during organic solvent diffusion. Typically, the thermal Marangoni effect results in fingering instability where the low interfacial tension difference and the drop curvature less than its spontaneous one allow that the flexible drop surface develops multiple undulations generating long fingers as the organic solvent diffuses towards the aqueous medium. In this process, the solvent carries polymer molecules into the aqueous phase. Then, if spontaneous curvature favors an organic phase-in water arrangement, it could be expected that many drops of smaller diameter detach from the fingers and
26 become dispersed in the aqueous phase. Thus new globules or polymer aggregates (not totally desolvated) are formed and stabilized by the stabilizing agent (protoparticles) which prevents their coalescence and the formation of agglomerates. The submicron particles will be formed after the complete diffusion of the solvent, if the stabilizing agent remains at the liquid–liquid interface during the diffusion process and if its protective effect is adequate. The mean nanocapsule size is always smaller than that of the emulsion droplets, in agreement with the diffusion theory proposed.
This technique presents several advantages, such as high encapsulation efficiencies, no need for homogenization, high batch- to-batch reproducibility, simplicity, and narrow size distribution.
Disadvantages are the high volumes of water to be eliminated from the suspension and the leakage of water-soluble drug into the saturated-aqueous external phase during emulsification, reducing encapsulation efficiency.
Double emulsions13 are complex heterodisperse systems called
“emulsions of emulsions”, that can be classified into two major types:
water-oil-water emulsion (w/o/w) and oil-water-oil emulsion (o/w/o). Thus the dispersed phase is itself an emulsion and the inner dispersed globule/ droplet is separated from the outer liquid phase by a layer of another phase. Double emulsions are usually prepared in a two-step emulsification process using two surfactants: a hydrophobic one designed to stabilize the interface of the w/o
27 internal emulsion and a hydrophilic one to stabilize the external interface of the oil globules for w/o/w emulsions. For preparation of nanocapsules, the principle of double emulsion formation, specifically of the w/o/w type, is associated with the principles of both nanoprecipitation and emulsion–diffusion methods. In this case, in the primary w/o emulsion the oil is changed by an organic phase containing a solvent that is totally or partially miscible in water, the film-formed polymer and a w/o surfactant. Then the water containing a stabilizing agent is added to the system to obtain the water in organic in water emulsion. However in this step, particle hardening is obtained through solvent diffusion and polymer precipitation. Water is frequently added to the double emulsion in order to achieve full solvent diffusion. The surfactants play a dual role in emulsions: as a film former and a barrier to drug release at the internal interface, and as a steric stabilizer on the external interface.
It was found that drug encapsulation efficiency and average particle size are affected by changing the type and concentration of both the w/o emulsion and the stabilizing agent. In a typical procedure for preparation of nanocapsules by double emulsification, the primary emulsion is formed by ultrasound and the w/o surfactant stabilizes the interface of the w/o internal emulsion.
The second emulsion is also formed by ultrasound and nanocapsule dispersion is stabilized by the addition of the stabilizing agent. Finally, the solvents are removed by evaporation or extraction by vacuum, leaving hardened nanocapsules in an aqueous medium.
28 Emulsion-Coacervation method
The emulsion-coacervation process is mainly presented as a strategy for nanocapsules preparation from naturally occurring polymeric materials. Up to now, sodium alginate and gelatin have been used though synthetic polymeric materials could be used for this purpose.
The procedure involves the o/w emulsification of an organic phase (oil, active substance and active substance solvent if necessary) with an aqueous phase (water, polymer, stabilizing agent) by mechanical stirring or ultrasound. Then, a simple coacervation process is performed by using either electrolytes14, by the addition of a water miscible non-solvent15 or a dehydration agent or by temperature modification16. Finally, the coacervation process is complemented with additional crosslinked steps that make it possible to obtain a rigid nanocapsule shell structure.
Nanocapsule formation by the emulsion-coacervation method uses the emulsion as a template phase and the formation of a coacervate phase that causes polymer precipitation from the continuous emulsion-phase to form a film on the template forming the nanocapsule. Additionally, it can be stabilized by physical intermolecular or covalent cross-linking, which typically can be achieved by altering pH or temperature, or by adding a cross-linking agent. Probably the critical stage in preparation of nanocapsules by the emulsion-coacervation method is coacervate phase formation17. In particular, the polymer dissolved in water is enclosed by water molecules that solvate its functional groups, typically through
29 hydrogen-bonding and van der Waals forces that prevent attraction among chain segments in close proximity by interchain H-bonds, or van der Waals or opposing ionic forces. Thus, the coacervating agents lower the solvation of dissolved polymers and induce thin solvated shell. It may also allow the attraction among contiguous chains via secondary valence bonds to form an entangled network or even non- covalent weak cross-links as the polymer concentration gradually increases in the coacervated phase. The use of electrolytes for polymer desolvation is known as salting-out. On the other hand, in the case where a dehydrating agent is used, the ternary system formed (polymer – dehydrating agent– water) allows the increase of polymer concentration due to solvent–solvation competition process.
This results in the desolvation of the polymer chains, leading to phase separation.
Polymer Coating method
In polymer coating method different methodological strategies can be used to deposit a thin layer of polymer on the nanoparticle surface. This can be achieved by adsorbing the polymer onto the preformed uncoated nanocapsules when the latter are incubated in polymer dispersion under predetermined stirring and time conditions18. Likewise, layer-formed polymer can be added during the final stage of conventional methods for the preparation of nanocapsules such as nanoprecipitation and double emulsification.
Thus, these methods have been modified in order to add a layer of polymer to the external aqueous medium and allow to simultaneous
30 layer formation due to the precipitation of the charged polymer (mainly negatively in nature) and to the diffusion of the solvent.
Another way is to prepare a nanoemulsion as template and then coat it by polymer deposition on the water/oil nanoemulsion surface. The polymers are added in the continuous phase and their precipitation onto the nanoemulsion droplets is triggered by solvent evaporation, as opposed to the emulsion coacervation method. For preparation of nanocapsules using this method an organic phase, composed of the active substance, oil, surfactant and solvent, and an aqueous phase containing the stabilizing agent and an aqueous polymer-coating solution are mixed under moderate stirring and the o/w nanoemulsion is formed by solvent displacement. The solvents are subsequently evaporated under vacuum until reaching a specific volume and the nanoemulsion is finally coated by the polymer by simple incubation in the polymer solution. The nanocapsule formation mechanism is mediated by the ionic interaction between surfactant and polymer.
The layer-by-layer assembly process developed for colloidal particle preparation makes it possible to obtain vesicular particles, called polyelectrolyte capsules, with well-defined chemical and structural properties19. To sum up, the mechanism of nanocapsule formation is based on irreversible electrostatic attraction that leads to polyelectrolyte adsorption at supersaturating bulk polyelectrolyte concentrations. This method requires a colloidal template onto which
31 is adsorbed a polymer layer either by incubation in the polymer solution, subsequently washed, or by decreasing polymer solubility by drop-wise addition of a miscible solvent. This procedure is then repeated with a second polymer and multiple polymer layers are deposited sequentially, one after another. It can be used as a template the solid form of the active substance, as can inorganic particles and biological cells. Likewise, the adsorption of oppositely charged polyelectrolytes can be done on the surface of colloidal particles with subsequent core dissolution. Also emulsion droplets, prepared by high-pressure homogenization, can be used as template.
Once the polyelectrolyte addition had ended, nanocapsule dispersion was again treated by high-pressure homogenization and the dispersion was finally centrifuged. The molecules employed for assembly should have a sufficient number of charged groups to provide stable adsorption on an oppositely charged surface and non- compensated charges exposed to the exterior. Furthermore, this method raises other difficulties such as the formation of counterions aggregates, the separation of the remaining free polyelectrolyte from the particles prior to the next deposition cycle and polyelectrolyte- induced bridging during centrifugation. Close particle–particle encounters may cause unfavorable interactions with the polyelectrolyte films, possibly leading to film destruction and aggregate formation. In addition, another difficulty is the particle sizes obtained which are higher than 500nm. Although these particle
32 sizes are at submicronic scale, they are obviously larger than the size commonly accepted for nanocapsules.
33 Thermally Induced Phase Separation (TIPS)
As explained in the previous paragraphs, nanocapsules of desired shape, composition and with tailored properties have exhibited potential applications of wide scientific and technological interest in the field of nanomedicine. However, methods applied in nanocapsular structure productions are still limited by several drawbacks, related to their production, such as high polidispersity index, low biocompability, poor feasibility of scaling-up to produce the cost reduction required to target markets, and time consuming procedures not suitable to be industrialized. Thus, the aim of this work is to overcome limitations of methods currently proposed in the fabrication of nanocapsules through several novel approaches.
In particular, most of the work involves Thermally Induced Phase Separation (TIPS) is a process based on the phenomenon that solvent effectiveness decreases when temperature is decreased20. Thus, when a homogeneous polymer solution at elevated temperature is cooled down, phase separation occurs, resulting in the formation of a polymer-rich phase and a polymer-lean phase. During the TIPS process the phase transitions may proceed in combinations with liquid–liquid phase separation and solidification such as vitrification, crystallization of the polymer, or freezing of the solvent. In most cases these solidifications are useful for fixing the structure of the solution at a certain stage during liquid–liquid phase separation.
Afterwards, the solvent can be removed by evaporation, freeze
34 drying, and extraction with non-solvents or critical point drying. The final morphology of the solution is determined by the extent of the liquid–liquid phase separation before solidification.
A typical phase diagram for a binary polymer solvent system is schematically represented in Fig .
Figure 3: A schematic representation of a binary phase diagram of a polymer solution showing a liquid-liquid demixing gap. In addition, the possible structure formation in the
different parts of the liquid-liquid demixing gap is indicated: nucleation and growth of polymer rich phase (left picture), bicontinuous morphology due tospinodal decomposition
(middle picture) and nucleation of a polymer poor phase (right picture).
In the figure the temperature is plotted as function of the polymer concentration. At higher temperatures the solution is still homogeneous, at lower temperatures liquid-liquid phase separation can take place. The miscibility gap can be divided into three areas.
The border of the miscibility gap is called the binodal, the dashed line is called the spinodal. Examples of compositions that are in
35 equilibrium are given by horizontal lines called tie lines. The point where the binodal and spinodal touch is called the critical point. At the critical point the polymer rich phase and the polymer poor phase have the same compositions. Compositions located between the binodal and the spinodal are metastable, this means that solutions are stable with respect to small composition fluctuations. However when the composition fluctuations are large enough phase separation will take place by nucleation and growth of a polymer poor phase in case the original composition of the solution is located at polymer concentrations lower than the critical point, resulting in a globular microporous structure. Likewise, the phase separation take place nucleation and growth of the polymer rich phase in case the polymer concentration is higher than the polymer concentration of the critical point, resulting in a cell-tunnel microporous structure.
Solutions quenched into the area enclosed by the spinodal are unstable. Any composition fluctuation can trigger a wave of composition fluctuations through the solution. The amplitude of the fluctuations will increase because the molecules of both components will move from low concentration regions to high concentration regions. In this case demixing usually yields network structures, in which both the polymer rich phase and the polymer poor phase are completely interconnected, forming a continuous structure. The spinodal area can only be entered directly at the critical point. In all other cases, the metastable area must first be passed. High cooling rates can be used to prevent demixing in the metastable area.
36 Up to now, Thermally Induced Phase Separation has extensively been used to fabricate foams, membranes and various porous biodegradable scaffolds suitable for tissue engineering and drug delivery. Here in, we demonstrate that by performing TIPS within nanoconfinement21 a transition to semicrystalline vesicular morphology can be observed for the first time and the formation of the uniform nanocapsules with controllable size and shell thickness can be obtained. This kind of architecture presents crystal properties, important features in the design and behavior of biocompatible, biodegradable and functionalized vectors, opening the way to the role of surface crystallinity of nanocapsular structures on several physicochemical aspects of interaction with a biological system. In particular, for this purpose we focused our research on Poly-L-Lactic Acid (PLLA), because it is a biopolymer largely studied by TIPS22; 23, generally producing two main types of morphology: globular-like and membrane-like. In our case, a mixture of dioxane and water was used for a binary composition of solvent and antisolvent respectively of the polymer. In particular, the ternary system PLLA/Dioxane/Water is a well-known UCST (Upper Critical Solution Temperature) system, for which several cloud point studies have already been reported in literature. Its binodal-spinodal diagram shows that the fundamental condition to perform our experiment is at low polymer concentration, where a solvent rich phase formation, as well as globular-like morphology, is favorite by decreasing temperature.
37 AIM OF THE WORK
In my PhD project I have focused my attention on Poly Lactic Acid because it is a synthetic polymeric material, already approved by The Food & Drug Administration on the basis of its good properties of non-toxicity, absolute biodegradability, adjustable degradation rate, and good biocompatibility24. In the first part of my work, I tried to take advantages by the Thermally Induced Phase Separation in order to control PLLA crystallization properties and to obtain for the first time nanocapsular morphology. Results were obtained by inducing phase transition of polymer chain in a nanoconfined domain. Later, I focused my attention on the tri-block copolymer made by PLA-PEG- PLA and I studied their micellization behavior in order to encapsulate contrast agents for Enhanced MRI. Last efforts were devoted to the combining of the previous processes to obtain nanostructures for application in the theranostic field. We envision polymer nanocapsules with cancer drug entrapped within the core, protected by a soft shell made by triblock copolymer containing contrast agents.
1 JANIB, S. M.; MOSES, A. S.; MACKAY, J. A. Imaging and drug delivery using theranostic nanoparticles. Advanced Drug Delivery Reviews, v. 62, n. 11, p. 1052-1063, Aug 30 2010.
ISSN 0169-409X. Disponível em: < <Go to ISI>://WOS:000285225200005 >.
2 CHO, K. et al. Therapeutic nanoparticles for drug delivery in cancer. Clinical Cancer Research, v. 14, n. 5, p. 1310-1316, Mar 1 2008. ISSN 1078-0432. Disponível em: < <Go to ISI>://WOS:000253565000007 >.
3 PEER, D. et al. Nanocarriers as an emerging platform for cancer therapy. Nature Nanotechnology, v. 2, n. 12, p. 751- 760, Dec 2007. ISSN 1748-3387. Disponível em: < <Go to ISI>://WOS:000251456500010 >.
4 BAO, G.; MITRAGOTRI, S.; TONG, S. Multifunctional Nanoparticles for Drug Delivery and Molecular Imaging.
Annual Review of Biomedical Engineering, Vol 15, v. 15, p.
253-282, 2013 2013. ISSN 1523-9829. Disponível em: < <Go to ISI>://WOS:000323896000012 >.
5 SWAMI, A. et al. Nanoparticles for Targeted and Temporally Controlled Drug Delivery. Multifunctional Nanoparticles for Drug Delivery Applications: Imaging, Targeting, and Delivery, p. 9-29, 2012 2012. Disponível em: < <Go to ISI>://WOS:000303542200002 >.
6 BAE, Y. H.; PARK, K. Targeted drug delivery to tumors: Myths, reality and possibility. Journal of Controlled Release, v. 153, n. 3, p. 198-205, Aug 10 2011. ISSN 0168-3659. Disponível em:
< <Go to ISI>://WOS:000295353800002 >.
7 HE, C. et al. Effects of particle size and surface charge on cellular uptake and biodistribution of polymeric nanoparticles.
Biomaterials, v. 31, n. 13, p. 3657-3666, May 2010. ISSN 0142-9612. Disponível em: < <Go to ISI>://WOS:000276254100027 >.
8 JOKERST, J. V. et al. Nanoparticle PEGylation for imaging and therapy. Nanomedicine, v. 6, n. 4, p. 715-728, Jun 2011. ISSN 1743-5889. Disponível em: < <Go to ISI>://WOS:000292994300019 >.
9 DE JONG, W. H.; BORM, P. J. A. Drug delivery and nanoparticles: Applications and hazards. International Journal of Nanomedicine, v. 3, n. 2, p. 133-149, 2008 2008. ISSN 1176-9114. Disponível em: < <Go to ISI>://WOS:000257848000002 >.
10 MORA-HUERTAS, C. E.; FESSI, H.; ELAISSARI, A. Polymer-based nanocapsules for drug delivery. International Journal of Pharmaceutics, v. 385, n. 1-2, p. 113-142, Jan 29 2010. ISSN 0378-5173. Disponível em: < <Go to ISI>://WOS:000274234100017 >.
11 ______. Influence of process and formulation parameters on the formation of submicron particles by solvent displacement and emulsification-diffusion methods Critical comparison.
Advances in Colloid and Interface Science, v. 163, n. 2, p. 90-
40 122, Apr 14 2011. ISSN 0001-8686. Disponível em: < <Go to ISI>://WOS:000290704600002 >.
12 QUINTANAR-GUERRERO, D. et al. Preparation and characterization of nanocapsules from preformed polymers by a new process based on emulsification-diffusion technique.
Pharmaceutical Research, v. 15, n. 7, p. 1056-1062, Jul 1998.
ISSN 0724-8741. Disponível em: < <Go to ISI>://WOS:000074897300017 >.
13 GARTI, N. Double emulsions - Scope, limitations and new achievements. Colloids and Surfaces a-Physicochemical and Engineering Aspects, v. 123, p. 233-246, May 15 1997. ISSN 0927-7757. Disponível em: < <Go to ISI>://WOS:A1997XG19000022 >.
14 LERTSUTTHIWONG, P. et al. Preparation of alginate nanocapsules containing turmeric oil. Carbohydrate Polymers, v. 74, n. 2, p. 209-214, Oct 16 2008. ISSN 0144- 8617. Disponível em: < <Go to ISI>://WOS:000258586700007
15 KRAUSE, H. J.; ROHDEWALD, P. Preparation of gelatin nanocapsules and their pharmaceutical characterization.
Pharmaceutical research, v. 2, n. 5, p. 239-43, 1985-Sep 1985.
ISSN 0724-8741. Disponível em: < <Go to ISI>://MEDLINE:24272844 >.
16 LUTTER, S. et al. Formation of gold nanoparticles in triblock terpolymer-modified inverse microemulsions. Colloids and Surfaces a-Physicochemical and Engineering Aspects, v. 329, n. 3, p. 169-176, Nov 5 2008. ISSN 0927-7757. Disponível em:
< <Go to ISI>://WOS:000260703400008 >.
17 ISHII, F.; TAKAMURA, A.; ISHIGAMI, Y. PROCEDURE FOR PREPARATION OF LIPID VESICLES (LIPOSOMES) USING THE COACERVATION (PHASE-SEPARATION) TECHNIQUE. Langmuir, v. 11, n. 2, p. 483-486, Feb 1995. ISSN 0743-7463. Disponível em: < <Go to ISI>://WOS:A1995QH98400020 >.
18 CALVO, P.; VILAJATO, J. L.; ALONSO, M. J. Evaluation of cationic polymer-coated nanocapsules as ocular drug carriers.
International Journal of Pharmaceutics, v. 153, n. 1, p. 41-50, Jul 16 1997. ISSN 0378-5173. Disponível em: < <Go to ISI>://WOS:A1997XL40100004 >.
19 SUKHORUKOV, G. B. et al. Layer-by-layer self assembly of polyelectrolytes on colloidal particles. Colloids and Surfaces a-Physicochemical and Engineering Aspects, v. 137, n. 1-3, p.
253-266, Jun 15 1998. ISSN 0927-7757. Disponível em: < <Go to ISI>://WOS:000074263400025 >.
20 VANDEWITTE, P. et al. Phase separation processes in polymer solutions in relation to membrane formation. Journal of Membrane Science, v. 117, n. 1-2, p. 1-31, Aug 21 1996. ISSN 0376-7388. Disponível em: < <Go to ISI>://WOS:A1996UZ77500001 >.
21 BINDER, K. et al. Confinement effects on phase behavior of soft matter systems. Soft Matter, v. 4, n. 8, p. 1555-1568, 2008 2008. ISSN 1744-683X. Disponível em: < <Go to ISI>://WOS:000260376800001 >.
22 TANAKA, T.; LLOYD, D. R. Formation of poly(L-lactic acid) microfiltration membranes via thermally induced phase separation. Journal of Membrane Science, v. 238, n. 1-2, p.
42 65-73, Jul 15 2004. ISSN 0376-7388. Disponível em: < <Go to ISI>://WOS:000222290900007 >.
23 CHEN, J.-S.; TU, S.-L.; TSAY, R.-Y. A morphological study of porous polylactide scaffolds prepared by thermally induced phase separation. Journal of the Taiwan Institute of Chemical Engineers, v. 41, n. 2, p. 229-238, Mar 2010. ISSN 1876-1070.
Disponível em: < <Go to ISI>://WOS:000276005400016 >.
24 GARLOTTA, D. A literature review of poly(lactic acid). Journal of Polymers and the Environment, v. 9, n. 2, p. 63-84, Apr 2001. ISSN 1566-2543. Disponível em: < <Go to ISI>://WOS:000177985700003 >.
41 CHAPTER II: NANOCAPSULES PRODUCTION BY THERMALLY INDUCED PHASE SEPRATION IN A NANOCONFINEMENT
Nanostructures were obtained through a novel approach based on Thermally Induced Phase Separation (TIPS) in nanoconfinement, that allows to obtain semicrystalline nanocapsules (down to 50 nm).Indeed, PLA is a slow-crystallizing material, and it is a hard challenge to succeed in inducing its crystallization in a TIPS process through the control of the main operating parameters. However, it is even more difficult to induce a nanoconfinement to produce semicrystalline PLLA nanocapsules by TIPS. Indeed, the prerequisites for a successful traditional TIPS process are (a) the complete miscibility between the liquid solvent and the antisolvent and (b) the insolubility of the solute in the antisolvent. So, in the approach that we are proposing, the idea was to follow the thermodynamic equilibrium of a standard ternary system with the peculiarity to induce the quenching phenomenon not in a macroscopic environment but in a single emulsion droplet, that we have called flexible nanoconfinement. For this purpose, we developed a new manufacturing process that takes advantages on the use of the innovative technology of High Pressure Homogenizer to produce very fine and more stable emulsions. Furthermore, this new process allows
42 producing stable, nanosized, biopolymer nanocapsules working in a continuous mode, with high throughput and in a cost effective way.
Poly,L-lactic acid (PLLA, Product name “ResomerTML 209 S”, with Mw = 12.5 KDa), was purchased by Evonik Industries.
Diethylene dioxide (1,4 – dioxane, anhydrous, purity 99.8%; density 1,034 g/ml at 25°C (lit.); molecular formula 𝐶4𝐻8𝑂2; 𝑀𝑤 = 88,11 𝑔 𝑚𝑜𝑙−1), Polyvinyl alcohol (PVA, linear formula [-CH2CHOH-]n, 𝑀𝑤 = 13000 − 23000 𝑔 𝑚𝑜𝑙−1), Pluronic F127 (PF127, powder, non- ionic, cmc: 950-1000 ppm ), Rhodamine B (molecular formula 𝐶28𝐻31𝐶𝑙𝑁2𝑂3; 𝑀𝑤 = 479.01 𝑔 𝑚𝑜𝑙−1, powder, purity≥95% (HPLC)), Gadolinium (III) Chloride (anhydrous, powder, 99.99% trace metals basis), Threalose dehydrate (molecular formula 𝐶12𝐻22𝑂11 ∙ 2𝐻2𝑂;
𝑀𝑤 = 378.33 𝑔 𝑚𝑜𝑙−1) were purchased by Sigma-Aldrich. Chromeo 488 Carboxylic Acid (molecular formula 𝐶30𝐻31𝑁𝑂7; 𝑀𝑤 = 517.58 𝑔 𝑚𝑜𝑙−1, reagent color: yellow-orange) was purchased by Active Motif.
The water, used as antisolvent for the polymer, was purified by distillation, deionization, and reserve osmosis (Milli–Q PLUS water purification system).
Poly - Lactic Acid (PLA)
Poly(lactic acid) (PLA) belongs to the family of aliphatic polyesters1; 2; 3. It can be produced by condensation polymerization directly from its basic building block lactic acid. The chiral nature of lactic acid results in
43 distinct forms of polylactide, namely, poly(L-lactide) (PLLA), poly(D- lactide) (PDLA), and poly(DL-lactide) (PDLLA), which are synthesized from the L-, D-, and DL-lactic acid monomers, respectively. The polymerization of racemic (D,L)-lactide however, results in the formation of amorphous polymers. Commercial PLA is usually prepared from L-lactide (LLA), because the resulting poly(L-lactic acid) (PLLA) is semicrystalline (~ 37% crystallinity) with a relatively high melting (175°C) and glass transition temperature (Tg = 60-65°C). The monomer LLA can be prepared with relatively high enantiopurity from corn starch fermentation. PLLA is a versatile, degradable polymer having excellent mechanical properties, good biocompatibility, and low toxicity, and is FDA approved. It has been used in a variety of applications in the pharmaceutical and biomedical fields, as well as used as a degradable plastic for disposable consumer products.
Processing, crystallization, and degradation behavior of PLA all depend on the structure and composition of the polymer chains, in particular on the ratio of the L- to the D-isomer of lactic acid4. PLLA is degraded by simple hydrolysis of the ester bond and does not require the presence of enzymes to catalyze this hydrolysis.
PROTOCOL FOR PLLA NANOCAPSULES PRODUCTION
Semicrystalline PLLA nanocapsules were produced in a cost effective and large quantity through an innovative Thermally Induced Phase
44 Separation (TIPS) approach starting by a preformed emulsion. Process has been performed in a continuous mode for preparing stable, dispensable, nanosized, biopolymer nanocapsules. A ternary solution of PLLA/water/Dioxane at a selected temperature ranging from 30 to 70°C was prepared. The components are added in an Erlenmeyer bulb, immersed in a silicone oil bath on a stirring hot plate, with a thermocouple used to control the oil bath temperature, set at 116°C, in order to allow the polymer to dissolve in the dioxane/water mixture.
The system is maintained at this temperature for at least 3 hours (depending on the polymer concentration) in continuous stirring (300 – 350 rpm), to facilitate the dissolution of the solid polymer pellets in solution and to keep the system homogeneity. The temperature of 116°C is higher than both the boiling points of dioxane (101°C) and water (100°C), so, during the dissolution of the polymer, evaporation of the low molecular weight species is expected, with consequent undesired change in system composition. To avoid this drawback, a glass Liebig condenser is installed on the top of the Erlenmeyer bulb containing the solution allowing condensing the vapors generated from heating the system, restoring the desired solution composition. After several hours, when the solution appears transparent, without stopping stirring, the system temperature is finally lowered at the preferred temperature and maintained at this value for at least one hour before starting the experiment, in order to stabilize the homogeneous solution obtained. The preformed solution was added to a continuous phase
45 containing a selected surfactant at the same temperature, with a surfactant concentration ranging from 0,5 to 3wt%, as required. This pre-emulsion was treated by ultrasonication (Branson Sonifier 450 cell disruptor) for 5 minutes at constant Temperature, controlled by a thermocouple. Then, the pre-emulsion is directly flowed in the High Pressure Homogenizer (Microfluidics M110P) with a Pressure ranging from 1000 to 2000 bar. After recirculating the emulsion for 10 minutes at high shear rate, the cooling steps has been performed. The emulsion was unloaded and kept under stirring at the same temperature, then directly injected in a custom-made hydrodynamic flow focusing system obtained by cold water at 5-6 °C. Inlet and outlet temperature were measured by a thermocouple. The obtained capsules were kept at 7-8 °C for at least 15 minutes up to 30.
Figure 1: Schematic representative of the process.
46 METHOD TO AVALUATE THE EFFECT OF COOLING RATE AND CONDITIONS ON THE SYSTEM
In order to evaluate the influence of quenching step, different kind of cooling methods have been applied on polymer solution, on pre- emulsion processed by ultrasonicator and on emulsion obtained by HPH, and different obtained morphologies have been observed. Protocols performed are listed below.
o Method I. Cooling at room temperature
Starting from the polymer solution at fixed polymer concentration, keeping ratio dioxane/water constantly at 87:13, cooling step has been performed by inducing the decreasing of the temperature leaving it at room temperature. The polymer solution temperature before the cooling step was always kept at 80°C.
o Method II. Cooling by water at room temperature
Starting from the polymer solution at fixed polymer concentration, keeping ratio dioxane/water constantly at 87:13, cooling step has been performed by inducing the decreasing of the temperature leaving it at room temperature and then injecting it in water at room temperature. The polymer solution temperature before the cooling step was always kept at 80°C.
o Method III. Cooling by cold water
47 Starting from the polymer solution at fixed polymer concentration, keeping ratio dioxane/water constantly at 87:13, cooling step has been performed by inducing the decreasing of the temperature injecting the solution in cold water. The polymer solution temperature before the cooling step was always kept at 80°C.
o Method IV. Cooling at room temperature starting from different temperatures
Starting from the polymer solution at fixed polymer concentration, keeping ratio dioxane/water constantly at 87:13, cooling step has been performed by inducing the decreasing of the temperature leaving it at room temperature, starting from different temperatures.
o Method I. Cooling by liquid nitrogen bath
Starting from the pre-emulsion at fixed polymer concentration, keeping ratio polymer/surfactant constantly at 1:2, cooling step has been performed by inducing the decreasing of the temperature immersing the pre-emulsion in a nitrogen bath.
Temperature was monitored at the beginning and at the end.
The pre-emulsion temperature before the injection was always kept at 80°C.
o Method II. Cooling by by Flow focusing